 Original Article
 Open access
 Published:
Optimization of production parameters of particle gluing on internal bonding strength of particleboards using machine learning technology
Journal of Wood Science volume 68, Article number: 21 (2022)
Abstract
The particleboard (PB) production is an extremely complex process, many operating parameters affecting panel quality. It is a big challenge to optimize the PB production parameters. The production parameters of particle gluing have an important influence on the internal bond (IB) strength of PB. In this study, using grey relation analysis (GRA) and support vector regression (SVR) algorithm, a prediction model was developed to accurately predict IB of PB through particle gluing processing parameters in a PB production line. GRA was used to analyze the grey relational grade between the particle gluing processing parameters and IB of PB, and the variables were screened. The SVR algorithm was used to train 724 groups of particle gluing sample data between six particle gluing processing parameters and IB. The SVR model was tested with 181 sets of experimental data. The SVR model was verified by 181 sets of experimental data, and the values of mean absolute error (MAE), mean relative error (MRE), root mean square error (RMSE), and Theil’s inequality coefficient (TIC) of the model were 0.008, 0.017, 0.013, and 0.014, respectively. The results showed that the prediction performance of the nonlinear regression prediction model based on GRA–SVR is superior, and the GRA–SVR prediction model can be used to realtime predict the IB in the PB production line.
Introduction
Particleboards (PB) have the characteristics of wide adaptability of raw materials and good mechanical properties, which has become one of the common boards in furniture manufacturing [1]. Threelayer particleboard is the most common PB, in which threelayer particles with different sizes are mixed with adhesive and hotpressed at a certain temperature [2]. In the production process, the mechanical properties of PB are the key evaluation indexes of its quality [3], and the internal bond (IB) strength is one of the most important mechanical characteristics [4].
By combining image analysis technology with the mathematical model, Dai et al. [5,6,7] found that the resin content and particle thickness and other parameters would change the particle surface glue cover rate, and the glue cover rate would affect the cohesive force between particles, resulting in the reduction in IB. In subsequent studies, the team established a mechanistic model for estimating IB of PB, and the prediction results showed that there was a nonlinear relationship between IB and resin content, particle dimensions, product density and other parameters [8]. Lin et al. [9] used single image multiprocessing analysis technology to obtain the edge photos of PB and found that there was a significant correlation between adhesive and IB, which could reflect the important influence of particle gluing production parameters on IB of PB. Based on the above studies, it can be seen that the production parameters of particle gluing have an important impact on IB of PB. However, due to the lack of theoretical guidance related to the production parameters of particle gluing, tuning its parameters can only be completed based on the actual experiences of workers, which is difficult to meet the accuracy of parameter regulation in the gluing process [10]. Using particle gluing parameters and IB to develop a nonlinear prediction model can improve the accuracy of parameter adjustment in particle gluing process, which is conducive to improving the quality of PB, stabilizing PB production, and provide theoretical guidance for the actual production of PB. Therefore, it is necessary to develop the prediction model of particle gluing parameters for IB of PB.
Young et al. [11] developed the prediction model of IB of the fiberboard based on quantile regression (QR), and the prediction results are better than those of the model developed by multiple linear regression (MLR). The results from the study could save the production cost of fiberboard. Therefore, it is particularly important to find a suitable method for particleboard modeling and prediction. In the past few decades, technological progress has been made in the international research on the influence of particle gluing production parameters on IB of PB. Haftkhani et al. [12] constructed a linear regression model based on pitheorem theory to predict IB of PB according to particle size, adhesive ratio, and other parameters, but the linear model could not effectively evaluate the nonlinear relationship between particle gluing production parameters and IB. Tiryaki et al. [13] established an artificial neural network (ANN) model to predict the effects of adhesive and compression time on IB of Oriental beech using polyvinyl acetate adhesives. The results showed that mean absolute percentage error between the predicted results of the ANN model and the experimental values was 2.5%. However, the ANN model training is timeconsuming and easy to fall into locally optimal solution [14]. Yang et al. [15] established a mathematical model between the mechanical properties of PB and 23 production process parameters of PB such as moisture content and glue amount based on principal component regression analysis and random forest (RF), and determined the relationship between the production process parameters of PB and the mechanical properties, such as IB and bending strength. However, under the coupling effect of various factors, excessive multidimensionality would lead to excessive fitting of the model, and it could limit the upper limit of prediction accuracy [16].
Support vector regression (SVR) is an application of support vector machine (SVM) to regression problems [17]. SVM is to solve the sample distance hyperplane maximization problem, and SVR principle transforms it into a structured risk minimization problem [18]. SVR can be applied to nonlinear model modeling, which has the advantages of simple structure and strong generalization ability [19,20,21], and it has successfully addressed the issues of regression forecasting in many areas. In terms of woodbased panels, Gao et al. [22] used SVR algorithm to establish a model to predict the fiber quality of medium density fiberboard with the parameters of conveyer screw revolution speed, accumulated chip height, and compared with the linear prediction model. The prediction results showed that the mean absolute error (MAE), mean relative error (MRE), root mean square error (RMSE) and Theil’s inequality coefficient (TIC) of the SVR model were reduced by 92.19%, 92.36%, 87.29% and 87.21% compared with the mixed logistic regression (MLR) linear prediction model. The excellent model prediction results show that SVR algorithm can be applied to the prediction of panel production parameters.
Grey relation analysis (GRA) mainly describes the relationship between the attributes of each variable by searching the Grey relational grade (GRG), and then determines the correlation degree of the influence of each variable on the target [23]. By utilizing GRA, the correlation between the production parameters of particle gluing and IB of PB was compared, and the production parameters with less correlation with IB of PB were screened out, so as to improve the upper limit of model prediction.
This study intended to establish the relationship between eight particle gluing production parameters including core particle discharge speed (f_{core}) in belt scale, surface particle discharge speed (f_{surface}) in belt scale, flow rate of core particle glue (v_{core}) from multipump dosing system, flow rate of surface particle glue (v_{surface}) from multipump dosing system, pressure on core particle gluing (p_{core}) from atomization spray head, pressure on surface particle gluing (p_{surface}) from atomization spray head, current for core particle gluing (I_{core}) in blender, and current for surface particle gluing (I_{surface}) in blender and IB of PB. First, by GRA, the production parameters with low correlation with IB were screened to improve the upper limit of model prediction. Second, the nonlinear regression prediction model of particle gluing production parameters and IB was established using SVR. Third, the prediction accuracy of the model was tested by comparing the predicted values with the experimental values. Finally, the influence of particle gluing production parameters on IB of PB was evaluated according to the model prediction results. Since the real PB production is an extremely complex process, it is a big challenge to optimize the PB production parameters. According to the literature review, this work is unique, because the relationships between particle gluing parameters and IB of PB were initially analyzed and controlled using GRA and SVR algorithms with a big data.
Experimental
Materials
In this study, the test data were collected in a real PB production line with an annual yield of 250,000 m^{3}. In this experiment, pine, fruit and miscellaneous wood were used as main raw materials to produce PB with a size of 2440 mm × 1550 mm × 18 mm. The produced PB without sanding and cooling process were examined and analyzed in this study.
In the production process, pine, fruit, and miscellaneous wood particles were mixed at a weight ratio of 2:2:1 for processing core and surface particles. The mixed raw wood materials were converted into core particles and surface particles through chipping, flaking, drying, screening and sifting processes, and then mixed with adhesives and other additives to conduct particle gluing. Among them, the urea–formaldehyde resins were used in the particleboard production. The temperature of the adhesive was maintained at about 25 °C before sizing, the potential of hydrogen value of the adhesive was maintained between 8.5 and 9.0, and the viscosity of adhesive measured to be 30–40 s at 25 ℃ using the T4 Viscosity Cup Method. The NDJ5 viscometer, produced by Lichen in China, was used in the T4 Viscosity Cup Method. The production parameters before particle gluing are shown in Table 1.
Experimental equipment, parameters, and testing
Main working process of gluing equipment
The main accessories and working principle of gluing equipment for core and surface particles are the same. The main components are shown in Fig. 1. The multipump dosing system (1) sends the adhesive to the atomization spray head (3) at a certain flow rate. By controlling the atomization spray head (3) using the air pressure pump (2), the adhesive is sprayed into the interior of the blender (4) in the form of “fog umbrella”. At the same time, the particles are continuously transported to the belt scale (5) then to the blender (4) for full gluing. Finally, the particles are discharged uniformly by the microcomputer controller (6).
In Fig. 1, the adhesive flow rate recorded by the multipump dosing system (1); the pressure value of atomization spray head (3) is shown by the pressure gauge on the air pressure pump (2); weighing and calculating particle feeding speed by the belt scale (5); the microcomputer controller (6) realtime displays the current in the blender (4).
Equipment parameters of blender
The blender used in the experiment was produced by IMAL–PAL, Italy. The internal picture of the blender is shown in Fig. 2, and blender parameters are listed in Table 2.
Test method
The IB of PB was tested by taking samples from plain PB after 48 h conditioning. The test method of IB in this study followed the standard of GB/T 17,657–2013 Test methods of evaluating the properties of woodbased panels and surface decorated woodbased panels [24]. The Mod.IB700 testing machine, produced by IMAL–PAL in Italy, was used in this study. The specimen with a size of 50 mm × 50 mm × 18 mm was placed in a conditioning chamber with a temperature of 20 ± 2 °C and a relative humidity of 65 ± 5% for equilibrating samples to a constant moisture content before the testing. The fracture specimen after IB tests is shown in Fig. 3.
To ensure that the relationship between the particle gluing production parameters and the IB of PB is not affected by the production parameters of other processes, the key production parameters of other processes after gluing are required to be constant or stable in a certain range. the 905 groups of sample data that meet the above requirements are used for modeling.
Methods
Grey relation analysis
GRA analysis process is to unify the data to an approximate range and calculate the grey relational grade between parameters through the data change trend of each parameter [25]. To reduce the absolute numerical difference of data caused by different dimensions of parameters, normalization is needed before the GRA analysis. Normalization usually uses min–max normalization or mean normalization in GRA [26]. This study selected the process of averaging data, as shown in the following equation:
where x(k) is a vector of normalized parameters, k is the k^{th} data in normalized parameters vector, \(\overline{x}\) is the mean value of data in normalized parameter vector. Grey relation analysis is shown in the following equation:
where \(x_{0} (k)\) is a vector of target parameters, \(x_{i} (k)\) is the i^{th} parameter vector, and ρ is discrimination coefficient, usually the smaller the resolution coefficient, the better the resolution, typically 0.5 [27].
Support vector regression algorithm
SVR has advantages in small sample, nonlinear and highdimensional pattern recognition [28]; therefore, SVR has excellent prediction effect between particle gluing production parameters and IB of PB.
Given a training sample set on \(T = \{ ({\varvec{x}}_{1} ,y_{1} ),({\varvec{x}}_{2} ,y_{2} ), \cdot \cdot \cdot ,({\varvec{x}}_{{\varvec{n}}} ,y_{n} )\}\) a feature space, where x_{i} ∈ R^{n} is the input sample vector, y_{i} ∈ R^{n} is the corresponding output sample, and n is the number of training data. Regression function as shown in the following equation:
where \(\omega \in R^{n}\) represents the weight vector, \(\varphi (x)\) represents the nonlinear mapping function, and b represents the deviation, so as to obtain the minimum structural risk of the regression function. The optimal solution of SVR regression problem can be obtained by introducing relaxation variable \(\xi_{i} \ge 0,\xi_{i}^{ * } \ge 0\) [29], as shown in Eqs. 4–5:
where C is the penalty factor, indicating the correlation between the empirical error of the model and the smoothness. ε is a prescribed parameter, and the Lagrange multiplier is used to solve the biobjective optimization problem. By introducing the Lagrange multiplier (\(a_{i}\) and \(a_{i}^{*}\)) [30], the regression function is obtained by dual solution as shown by Eq. 6,
Introducing \(\varphi (x)^{T} \varphi (x)\) in the kernel function \(K(x_{i} ,x_{j} )\) substitution, as shown by Eq. 7,
Since the Gaussian Radial Basis Function (RBF) has good generalization, nonlinear prediction performance and less adjustment parameters [31], this paper selects RBF as the kernel function. RBF function as shown by Eq. 8,
To improve the prediction accuracy of the model, it is necessary to optimize the penalty coefficient “C” and the width of Gaussian RBF kernel “σ” [32]. In this paper, the 5folder crossvalidation was used to conduct grid search the training set samples.
The GRA–SVR prediction model for IB
Step 1: GRA correlation analysis
Through the GRA analysis of f_{core}, f_{surface}, v_{core}, v_{surface}, p_{core}, p_{surface}, I_{core} and I_{surface} on the grey relational grade of IB, the variables with low grey relational grade were screened out.
Step 2: Normalization of sample data
The normalization of sample data was to scale the data in the interval [0, 1], remove the unit limitation of sample data, and transform it into dimensionless pure values, so that different units can be maintained stable in the training process of the SVR model.
Step 3: Optimization of grid search parameters by Kfold cross validation
The grid search trains all the candidate parameters by the exhaustive method. Combined with the Kfold cross validation, the sample data set of the validation set was divided into k subsets and each subset performed the validation set once. The subset was used as the training set, and the validation K times were trained repeatedly until the penalty coefficient “C” of the minimum mean square error and the width “σ” of the Gaussian RBF kernel were selected as the optimal parameters.
Step 4: Constructing SVR nonlinear prediction model
The SVR prediction model for IB was established through the determined optimal parameters, and the model can predict each input. The SVR prediction models imported from the training set and the testing set were, respectively, used for prediction. The predicted values of the model output were compared with the experimental values, and the deviation of the model prediction was analyzed. The GRA–SVR prediction model diagram, as shown in Fig. 4.
Step 5: Evaluation of GRA–SVR model
MAE, MRE, RMSE and TIC were used to analyze the convergence of predicted values of GRA–SVR model to experimental values, and then the prediction performance of the model was accurately evaluated.
Results and discussion
Grey relation analysis production parameters of particle gluing
The grey relational grade results of particle gluing production parameters of f_{core}, f_{surface}, v_{core}, v_{surface}, p_{core}, p_{surface}, I_{core} and I_{surface} on IB calculated by GRA are shown in Fig. 5. The order of correlation between the production parameters of particle gluing and the IB of PB can be obtained intuitively: v_{core} > f_{core} > p_{core} > p_{surface} > v_{surface} > f_{surface} > I_{core} > I_{surface}.
On the one hand, the grey relational grades of v_{core}, f_{core} and p_{core} on IB were 0.773, 0.771 and 0.745, respectively, which are higher than that of p_{surface}, v_{surface} and f_{surface} on IB. It can be proved that the production parameters of core particle gluing have higher influence on the IB of PB than that of surface particle gluing. On the other hand, because the grey relational grades of I_{core} and I_{surface} to IB were 0.697 and 0.697, respectively, which were far lower than other production parameters, it was proved that I_{core} and I_{surface} had little effect on IB. The input of these two parameters into SVR regression prediction model for training would lead to lower prediction accuracy of the model. Therefore, only parameters of f_{core}, f_{surface}, v_{core}, v_{surface}, p_{core} and p_{surface} were taken into account for the training of the SVR model.
Regression prediction of GRA–SVR algorithm
The prediction model of particle gluing process parameters and IB using GRA–SVR was trained. The input variables were f_{core}, f_{surface}, v_{core}, v_{surface}, p_{core}, p_{surface}, and the output variable was IB. The total experimental data obtained by the experiment was 905 groups, of which 724 groups of data were used as a training set to build the model and 181 groups of data as a validation set to verify the model. SVR parameters were optimized by 5CV. The penalty coefficient “C” was 0.71, and the width “σ” of Gaussian RBF kernel was 8. Figure 6 shows that the prediction IB values obtained by the training set into the nonlinear regression prediction model were compared with the experimental values. The predicted values of the model in the image were highly consistent with the experimental values, which proved that the model had appealing fitting.
To accurately evaluate the prediction accuracy of the nonlinear prediction model of particle gluing production parameters and IB, the scatter distribution of the predicted and experimental values of the training set and the testing set was plotted using the image analysis model as shown in Fig. 7. If the predicted values of the model match the experimental values completely, all data points would be on the main diagonal. Figure 7a shows that the sample points of the training set and the testing set are very close to the main diagonal. Figure 7b shows that the relative deviation between the predicted values and the experimental values are small. It is indicated that the IB of PB model using GRA–SVR has good prediction accuracy.
As shown in Fig. 8, 91.16% testing data were within the 0–10% relative deviation between the predicted values and the experimental values, 28.28% testing data were ranged from 10 to 20% relative deviation, and 0.55% testing data were in 20–30% relative deviation. It was shown that the GRA–SVR prediction model of IB of PB had excellent accuracy.
Prediction performance evaluation of GRA–SVR algorithm
As shown in Fig. 8, although the GRA–SVR model had high accuracy, there was still 8.83% of the relative deviation of the predicted value between 10 to 30%. In addition to the nonlinear model itself, the error of data collection would also affect the accuracy of the model. Dai et al. [33] believed that vertical density profile (VPD) had a great influence on the IB of PB. Jin et al. [34] explored the regression relationship between IB and density of PB through the laminated beam theory, and the results showed that there was a positive correlation between IB and density of PB.
To explore the influence of VPD of PB on the prediction accuracy of GRA–SVR model, this study conducted six VPD tests on a randomly selected specimen, and the results are shown in Fig. 9. It could be seen from the figure that with the increase of PB thickness, the variation trend of density in the vertical direction was a profile of ’M’. The density variation trend of the middle layer of PB was relatively flat, but there was still ± 30 kg/m^{3} density fluctuation. Because the density of particleboard was positively correlated with IB, if the fracture position of the specimen changes during IB tests, it would lead to the deviation of IB test results. This indicates that the more uniform density of PB intermediate layer, the higher the accuracy of GRA–SVR model can be achieved.
The training set sample data and the testing set sample data were inputted into the model for prediction, and MAE, MRE, RMSE, and TIC were used to evaluate the prediction performance of the model. As shown in Table 3, the results showed that the model errors were small, indicating the model had good prediction performance.
Application of the GRA–SVR model
Manufacturers would change PB production according to different order requirements. The particle discharge speed in the belt scale in the particle gluing process would change with the change of PB yield. The GRA–SVR model in this study could change the production parameters of particle gluing according to the actual production demand, so as to improve the IB of PB.
Assuming that f_{core} was adjusted to 325 kg/min to meet the production demand of PB, the production parameters of particle gluing are predicted. The range of particle gluing production parameters is shown in Table 4. The prediction process took f_{core} = 325 kg/min as a constant, and the other five production parameters used 100 as the step length to bring into the GRA–SVR model for the grid search optimization. When the value of particle gluing production parameters was f_{surface} = 154.1 kg/min, v_{core} = 37.5 L/min, v_{surface} = 27 L/min, p_{core} = 1.9 bar, p_{surface} = 1.8 bar, the optimal value of IB of PB was 0.55 MPa.
On the other hand, PB manufacturers would reduce production costs by reducing adhesive consumption according to the actual situation of orders. Reducing the adhesive consumption of PB would lead to the decrease of IB [35]. The GRA–SVR model was used to predict the production parameters of particle gluing after reducing the flow rate of the particle glue from multipump dosing system, which could ensure the production of PB under the minimum IB for meeting the enterprise standards. Therefore, the modeling and optimization of particle gluing processing parameters and IB of PB are conducive to reducing the production cost of PB and improving the quality of products.
Conclusions
In this study, a nonlinear regression prediction model between particle gluing processing parameters and IB of PB was developed using GRA–SVR. The six input parameters of f_{core}, f_{surface}, v_{core}, v_{surface}, p_{core} and p_{surface} were used to predict IB, which can quantitatively evaluate the influence of particle gluing production parameters on IB of PB and provide a new method for particle gluing process.
(1) GRA was used to analyze the grey relational grade between the particle gluing parameters of f_{core}, f_{surface}, v_{core}, v_{surface}, p_{core}, p_{surface}, I_{core} and I_{surface} and IB of PB. The results showed that the core particle gluing parameters had a higher proportion of the influence on the IB strength compared with the surface particle gluing parameters. I_{core} and I_{surface} had smaller influence on IB compared with other parameters.
(2) The predicted IB values obtained using the nonlinear regression prediction model were compared with experimental values. The results showed that the predicted values were in good agreement with the experimental values, and the relative deviations of 91.16% data points were in the range of 0–10%, indicating that the particle gluing model using GRA–SVR had satisfactory regression prediction accuracy.
(3) The sample data of training set were used by the GRA–SVR nonlinear regression prediction model to predict particleboard IB and the production parameters of particle gluing. The evaluation results showed that MAE was 0.004, MRE was 0.008, RMSE was 0.011, and TIC was 0.011, proving that the GRA–SVR model had good fitting. The GRA–SVR regression prediction model was used to predict the testing set sample data. The evaluation results showed that MAE was 0.008, MRE was 0.017, RMSE was 0.013, and TIC was 0.014, proving that the application of GRA–SVR model has excellent accuracy.
Using the GRA–SVR regression prediction model, IB of PB can be predicted in real time according to the production parameters of particle gluing. The manufacturers would adjust particle discharge speed in the belt scale and flow rate of particle glue from multipump dosing system in the process of particle gluing according to the actual production demands, so as to improve the yield of PB or reduce the adhesive consumption. The GRA–SVR model was used to predict the production parameters of particle gluing after the adjustment, so that the IB of PB meets the requirements of enterprise standards. The GRA–SVR modeling and prediction are helpful to guide the production practice of particleboards and has promising application future for efficient and stable production in the particleboard manufacturing industry.
Availability of data and materials
The data sets used and analyzed during the current study are available from the corresponding author upon reasonable request.
Abbreviations
 IB:

Internal bond strength
 PB:

Particleboards
 GRA:

Grey relation analysis
 SVR:

Support vector regression
 MAE:

Mean absolute error
 MRE:

Mean relative error
 RMSE:

Root mean square error
 TIC:

Theil’s inequality coefficient
 MLR:

Mixed logistic regression
 ANN:

Artificial neural network
 f _{core} :

Core particle discharge speed in belt scale
 f _{surface} :

Surface particle discharge speed in belt scale
 v _{core} :

Flow rate of core particle glue from multipump dosing system
 v _{surface} :

Flow rate of surface particle glue from multipump dosing system
 p _{core} :

Pressure on core particle gluing from atomization spray head
 p _{surface} :

Pressure on surface particle gluing from atomization spray head
 I _{core} :

Current for core particle gluing in blender
 I _{surface} :

Current for surface particle gluing in blender
 VPD:

Vertical density profile
References
Hansted FAS, Hansted ALS, Padilla ERD, Caraschi JC, Goveia D, de Campos CI (2019) The use of nanocellulose in the production of medium density particleboard panels and the modification of its physical properties. BioResources 14(3):5071–5079. https://doi.org/10.15376/biores.14.3.50715079
Yuan M, Hong L, Ju ZH, Gu WL, Shu BQ, Cui JX (2021) Structure design and properties of threelayer particleboard based on high voltage electrostatic field (HVEF). J Renew Mater 9(8):1433–1445. https://doi.org/10.32604/jrm.2021.015040
Huang HK, Hsu CH, Hsu PK, Cho YM, Chou TH, Cheng YS (2020) Preparation and evaluation of particleboard from insect rearing residue and rice husks using starch/citric acid mixture as a natural binder. Biomass Convers Biorefinery. https://doi.org/10.1007/s13399020009946
de Palacios P, Femandez FG, GarciaIruela A, GonzalezRodrigo B, Esteban LG (2018) Study of the influence of the physical properties of particleboard type P2 on the internal bond of panels using artificial neural networks. Comput Electron Agric 155:142–149. https://doi.org/10.1016/j.compag.2018.10.012
Dai CP, Yu CM, Zhou C (2007) Theoretical modeling of bonding characteristics and performance of wood composites. Part I. Interelement contact. Wood Fiber Sci 39(1):48–55
Dai CP, Yu CM, Groves K, Lohrasebi H (2007) Theoretical modeling of bonding characteristics and performance of wood composites. Part II. Resin distribution. Wood Fiber Sci 39(1):56–70
He G, Yu C, Dai C (2007) Theoretical modeling of bonding characteristics and performance of wood composites. Part III. Bonding strength between two wood elements. Wood Fiber Sci 39(4):566–577
Dai CP, Yu CM, Jin JW (2008) Theoretical modeling of bonding characteristics and performance of wood composites. Part IV. Internal bond strength. Wood Fiber Sci 40(2):146–160
Lin H, Huang J (2004) Using single image multiprocessing analysis techniques to estimate the internal bond strength of particleboard. Taiwan J 19(2):109–117. https://doi.org/10.7075/TJFS.200406.0109
Andre N, Young TM (2013) Realtime process modeling of particleboard manufacture using variable selection and regression methods ensemble. Eur J Wood Wood Prod 71(3):361–370. https://doi.org/10.1007/s0010701306890
Young TM, Shaffer LB, Guess FM, Bensmail H, Leon RV (2008) A comparison of multiple linear regression and quantile regression for modeling the internal bond of medium density fiberboard. For Prod J 58(4):39
Haftkhani AR, Arabi M (2013) Improve regressionbased models for prediction of internalbond strength of particleboard using Buckingham’s pitheorem. J For Res 24(4):753–740. https://doi.org/10.1007/s1167601304123
Tiryaki S, Bardak S, Bardak T (2015) Experimental investigation and prediction of bonding strength of Oriental beech (Fagus orientalis Lipsky) bonded with polyvinyl acetate adhesive. J Adhes Sci Technol 29(23):2521–2536. https://doi.org/10.1080/01694243.2015.1072989
Hong WC, Dong YC, Zhang WY, Chen LY, Panigrahi BK (2013) Cyclic electric load forecasting by seasonal SVR with chaotic genetic algorithm. Int J Electr Power Energy Syst 44(1):604–614. https://doi.org/10.1016/j.ijepes.2012.08.010
Yang CP, Xu C, Su JL, He W, Gao ZH (2021) A new model based on principal component regressionrandom forest for analyzing and predicting the physical and mechanical properties of particleboard. BioResources 16(2):2448–2471. https://doi.org/10.15376/biores.16.2.24482471
Rezaali M, Quilty J, Karimi A (2021) Probabilistic urban water demand forecasting using waveletbased machine learning models. J Hydrol. https://doi.org/10.1016/j.jhydrol.2021.126358
Cortes C, Vapnik V (1995) Supportvector networks. Mach Lean 20:273–297
Chang CC, Lin CJ (2011) LIBSVM: a library for support vector machines. ACM Trans Intell Syst Technol. https://doi.org/10.1145/1961189.1961199
Wang DC, Wang MH, Qiao XJ (2009) Support vector machines regression and modeling of greenhouse environment. Comput Electron Agric 66(1):46–52. https://doi.org/10.1016/j.compag.2008.12.004
Sun ZG, Wang CX, Niu XM, Song YD (2016) A response surface approach for reliability analysis of 2.5D C/Si C composites turbine blade. Composites Part B Eng 88:277–285. https://doi.org/10.1016/j.compositesb.2015.09.025
Zhou Z, Yin JX, Zhou SY, Zhou HK, Zhang Y (2016) Detection of knot defects on coniferous wood surface using near infrared spectroscopy and chemometrics. BioResources 11(4):9533–9546. https://doi.org/10.15376/biores.11.4.95339546
Gao YB, Hua J, Chen GW, Cai LP, Jia N, Zhu LK (2018) Prediction of fiber quality using refining parameters in mediumdensity fiberboard production via the support vector machine algorithm. BioResources 13(4):8184–8197. https://doi.org/10.15376/biores.13.4.81848197
Xiao XP, Deng JL (2001) A new modified GM (1,1) model: grey optimization model. J Syst Eng Electron 12(2):1–5
General administration of quality supervision, inspection and quarantine of the people 's republic of China, China national standardization management committee (2014) Test methods of evaluating the properties of woodbased panels and surface decorated woodbased panels: GB/T 17657–2013. Beijing: Standards press of China, 2014.04.11
Senthilkumar S, Karthick A, Madavan R, Moshi AAM, Bharathi SRS, Saroja S, Dhanalakshmi CS (2021) Optimization of transformer oil blended with natural ester oils using Taguchibased grey relational analysis. Fuel. https://doi.org/10.1016/j.fuel.2020.119629
Wei GW, Lei F, Lin R, Wang R, Wei Y, Wu J, Wei C (2020) Algorithms for probabilistic uncertain linguistic multiple attribute group decision making based on the GRA and CRITIC method: application to location planning of electric vehicle charging stations. Econ Res Ekonomska Istrazivanja 33(1):828–846. https://doi.org/10.1080/1331677X.2020.1734851
Sarikaya M, Gullu A (2015) Multiresponse optimization of minimum quantity lubrication parameters using Taguchibased grey relational analysis in turning of difficulttocut alloy Haynes 25. J Clean Prod 91:347–357. https://doi.org/10.1016/j.jclepro.2014.12.020
Baydaroglu O, Kocak K (2014) SVRbased prediction of evaporation combined with chaotic approach. J Hydrol 508:356–363. https://doi.org/10.1016/j.jhydrol.2013.11.008
Santos CED, Sampaio RC, Coelho LD, Bestard GA, Llanos CH (2021) Multiobjective adaptive differential evolution for SVM/SVR hyperparameters selection. Pattern Recogn. https://doi.org/10.1016/j.patcog.2020.107649
Shi F, Wang XC, Yu L, Li Y (2020) 30 case analysis of MATLAB neural network. Beihang University Press, Beijing
Zhao YS, Zhao JH, Huang Y, Zhou Q, Zhang XP, Zhang SJ (2014) Toxicity of ionic liquids: database and prediction via quantitative structureactivity relationship method. J Hazard Mater 278:320–329. https://doi.org/10.1016/j.jhazmat.2014.06.018
Guzman SM, Paz JO, Tagert MLM, Mercer AE, Pote JW (2018) An integrated SVR and crop model to estimate the impacts of irrigation on daily groundwater levels. Agric Syst 159:248–259. https://doi.org/10.1016/j.agsy.2017.01.017
Dai CP, Yu CM, Hubert P (2000) Modeling vertical density profile in wood composites during hotpressing. In: Proceedings of the 5th Pacific Rim Biobased Composites Symposium, Canberra, Australia,1013 December 2000, pp 220226.
Jin JW, Dai CP, Hsu WE, Yu CM (2009) Properties of strand boards with uniform and conventional vertical density profiles. Wood Sci Technol 43(7–8):559
Gu K, Li KC (2011) Preparation and evaluation of particleboard with a soy flourpolyethyleniminemaleic anhydride adhesive. J Am Oil Chem Soc 88(5):673–679. https://doi.org/10.1007/s1174601017067
Acknowledgements
The authors are grateful for the support of the Fundamental Research Funds for the Central Universities
Funding
This research was supported by the Fundamental Research Funds for the Central Universities, Grand No. 2572020AW42.
Author information
Authors and Affiliations
Contributions
BZ analyzed the experimental data and drafted the manuscript. JH is the project leader and responsible for the experimental design and manuscript review. LC responsible for manuscript review and language editing. YG checked algorithm prediction results. YL assisted the experiments.
Corresponding author
Ethics declarations
Competing interests
The authors declare that they have no competing interests.
Additional information
Publisher's Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this licence, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Zhang, B., Hua, J., Cai, L. et al. Optimization of production parameters of particle gluing on internal bonding strength of particleboards using machine learning technology. J Wood Sci 68, 21 (2022). https://doi.org/10.1186/s10086022020292
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/s10086022020292